copper-tin anodes for rechargeable lithium batteries: by ...€¦ · copper-tin anodes for...
Embed Size (px)
Copper-Tin Anodes for Rechargeable Lithium Batteries:An Example of the Matrix Effect in an Intermetallic System
K. D. Kepler, J. T. Vaughey, and M. M. Thackeray @ ~ ~Electrochemical Technology Program
Chemical Technology DivisionGOg@
Argonne National Laboratory “+g$
Argonne, IL U.S.A. u
The submitted manuscript has been created by theUniversity of Chicago as Operator of Argonne NationalLaboratory ~Argonne”) under Contract No.W-31-109-ENG-38 with the U.S. Department of Energy.The U.S. Government retains for itself, and others actingon its behalf, a paid-up, nonexclusive, irrevocableworldwide license in said article to reproduce, preparederivative works, distribute copies to the public, andperform publicly and display publicly, by or on behalf ofthe Government.
To be presented at the 9th International Meeting on Lithium Batteries, Edinburgh, Scotland,United Kingdom, July 12-17,1998
...- --- --— -—..—. . ———.. .— -. . . ..
This repofi was prepared as an account of work sponsoredby an agency of the United States Government. Neither theUnited States Government nor any agency thereof, nor any .of their employees, make any warranty, express or implied,or assumes any legal liability or responsibility for theaccuracy, completeness, or usefulness of any information,apparatus, product, or process disclosed, or represents thatits use would not infringe privately owned rights. Referenceherein to any specific commercial product, process, orservice by trade name, trademark, manufacturer, orotherwise does not necessarily constitute or imply itsendorsement, recommendation, or favoring by the UnitedStates Government or any agency thereof. The views andopinions of authors expressed herein do not necessarilystate or reflect those of the United States Government orany agency thereof.
Po~ions of this document may be illegiblein electronic image products. Images areproduced from the best available originaldocument.
Copper-Tin Anodes for Rechargeable Lithium Batteries:
An Example of the Matrix Effect in an Intermetallic System
K. D. Kepler, J. T. Vaughey, and M. M. Thackeray*
Electrochemical Technology Program
Chemical Technology Program
Argonne National Laboratory
Argonne IL 60439
Keywords: lithium battery, anode, intermetallic, tin alloy
Lithium batteries are typically constructed from a lithium cobalt oxide cathode and a
carbon anode. We have investigated intermetallic anode materials based on tin, which
can provide a high capacity at a slightly higher voltage (400 mV) than metallic lithium
and thus reduce the safety concerns associated with the carbon anode. In particular, we
have investigated the copper-tin system at around the composition CufjSns and have
determined the effect on cycling and capacity of electrodes with various ratios of copper
to tin. Anode compositions that are slightly copper rich (Cu&h@ were found to exhibit
greater utilization of the tin than those with the stoichiometric bronze ratio (Cu@@ or
those having a slight excess of tin (Curj&kj). The differences in electrochemical behavior
are explained in terms of an inert matrix model.
* Correspondingauthor, email:[email protected]: Tele: (630)-252-9184 Fax (630)-252-4176
.L. ,,..- . . .—
. . . .
Lithium batteries represent an important area of study and a developing market for
commercial batte~ companies. Conventional lithium-ion cells are constructed from a
lithium cobalt oxide cathode and a carbon anode. When graphite is used, this
electrochemical couple provides a voltage of approximately 4 V. There is some concern
about the cost of the cathode, irreversible capacity losses with cycling and safety of the
anode . We have been searching for alternative anode materials to carbon and have
been investigating interrnetallic materials based on tin which provide a high capacity at a
slightly higher voltage (400 mV) than metallic lithium, thus reducing safety concerns.
It is known that although the capacity of pure tin is high (990 mAh/g), it has a
limited cycle life. This has been attributed to a number of causes, including electronic
isolation of the lithiated product and poor electrical contact with the current collector
caused by the frequent expansion/compression cycles associated with the Mhiation . It
has been suggested that isolating the tin within a host matrix would solve many of these
problems . One of the more recently publicized methods was reported by Fujifdm
Celltec. They successfully loaded tin oxide (SnO) into a porous borophosphate glass, and
were able to demonstrate high capacity and low fade with cycling . Later reports by
Courtney and Dahn  indicated that the reaction mechanism involved the decomposition
of the tin oxide to tin metal and a subsequent alloying reaction with lithium. Although
under certain conditions the tin oxide was shown to be a stable anode system, problems
with an initial large irreversible capacity have limited its effectiveness. An alternative to
the oxide precursor is to use a tin intermetallic compound that does not require the
reduction of tin oxide (producing irreversible capacity). We have chosen to investigate
interrnetallic compounds in the copper tin system because they are easy to synthesize,
stable in an air environment, and because structural decomposition would encase the
lithiurnhin alloy in a conductive copper matrix. Here, we report our work on alloy
compositions at and around the s-bronze @$n5.
Three compositions were synthesized in the copper-tin system: @$ns, @$h&
and @Sn& The copper tin interrnetallics were synthesized by direct reaction of the
elements. Elemental copper (Johnson Mathey 99.9%) and tin (Aldrich, 99.8%) powder
were mixed in a stoichiometric ratio to yield the desired product. The mixed powders
were then pressed into a pellet, placed into an alumina crucible, and heated under an
argon atmosphere at 400 “C for 12 hr. The gray brittle product was then ground and
sifted to approximately 400 mesh. X-ray diffraction analysis of the product gave the
expected product distribution in each case. The stoichiometric bronze Cu&hs was a
single phase, the composition Cu&u gave a mixture of copper and the bronze, while the
COITIpOSitiOII cu(fhfj gave the bronze plus tin.
Additionally, we synthesized the lithium-copper-tin Zintl phase, LizCuSn
(MnCu2A1-type), as a lithiated precursor to Curjsns. Elemental lithium, copper, and tin
were weighed out in stoichiometric amounts and placed in a tantalum tube,, one end of
which had been crimped shut to forma metal test tube. The sample was heated to 900”C
under an argon atmosphere, held for three hours, and cooled radiatively to room
temperature. The violet-purple sample was then isolated from the tube as a powder. X-
ray analysis of the sample confined the isolation of the desired phase .
Laminates of the alloy materials and pure tin were evaluated in 1225 coin cells vs.
Li metal. The electrolyte used was 1 M LipFG in ethylene carbonate/diethyl carbonate
(50:50). The positive electrode laminates were made by doctor blading slurries
containing approximately 6 mg of active copper-tin material (81$%by mass), mixed with
carbon (XC-72, 9% by mass) and binder (Kynar 2801, 10% by mass) in tetrahydrofuran
(THF). The air-sensitive Li2CuSn laminates were made in a glove box. Cell construction
is described elsewhere . Cells were discharged and charged at constant current (O.1
mA) between either 1.2 and 0.0 V, or 1.2 and 0.2 V.
Results and Discussion
The idea of using an inert matrix to shield a battery anode was proposed by
Huggins a number of years ago . We have investigated the use of intermetallic alloys
as anodes, termed M’M, where M’ is an inactive metal and M is the component that
alloys with lithium. In this paper, the specific intermetzdlic we have chosen to
concentrate on is the E-bronze compound @Sns. Lithium insertion directly into this
compound is not possible because it lacks an interstitial site for the extra cation and has a
closed electronic configuration. The structure is shown in Fig. 1. Thus, any reaction with
lithium must happen by a displacement reaction and a breakdown of the starting bronze
compound to form copper (the inactive component) and tin. Further lithiation of the
system forms a series of lithium tin alloys (LiXSn,0cxs4.4) that follows the known phase
diagram. It is this tin that provides the anode capacity, while the displaced copper,
dispersed into the solid, acts as an electronically conducting matrix. It is envisioned that
this matrix will mitigate some of the unwanted expansion and contraction observed in
lithium alloy systems.
In our experiments, the three samples synthesized had the Compositioncu6sn5+8
(3= O,+1). The sample with 6 = Ois the single-phase bronze, the sample with 6 = 1 has
excess tin in the starting material, and the sample with 6 = -1 has an excess of copper.
Fig. 2(a and b) shows the voltage profile for Li/Sn and L~cU6&15 cells. All cells with
Cu-Sn anodes had profiles similar to pure tin and exhibited a distinct voltage plateau
around 400 mV versus lithium, corresponding in the phase diagram to Li7Sn3. All of the
Cu-Sn cells cycled better than our pure tin cells prepared in the same manner (Fig. 3).
Interestingly, we found that the greater the amount of Cu in the alloy, the better the
utilization of the tin. Thus, @Su exhibited the highest capacity per mass of tin present
(Fig. 4). We believe that this effect is related to the microstructure produced during the
initial decomposition of the alloy, which should lead to finely divided tin in an inactive
copper matrix. The additional Cu might lead to more finely divided tin, and the high
surface area of the tin could be accessible to Li through grain boundary diffusion. The
capacity fade of the Cu-Sn materials was slightly less than that of pure tin, suggesting that
the presence of a Cu matrix has only partially decreased the swelling problems. The
addition of more Cu might help the cycle life but at the expense of cell capacity. The
capacity retention was improved by changing the lower voltage cutoff to 200 mV, though
with a loss of cell capacity (Fig. 5).
We also investigated the lithium copper tin Zintl phase, LizCuSn, shown
schematically in Fig. 6. For this compound, besides the initial delithiation, the cycling
profile is similar to that observed for @$ns (Fig. 2c). Interestingly, the delithiation of
Li2CuSn at -800 mV is 400 mV greater than the potential for the delithiation of LiTSns,
the Li-Sn phase with the closest lithium to tin ratio. This suggests that the addition of Cu
to the metal framework stabilizes the Sn to oxidation. In the LizCuSn cells, the cell
capacity was well below the expected value of - 650 rnAh/g (Fig. 3), which we partly
ascribe to the electrical isolation of a large portion of the material during processing as
the compound reacted with air “to form LizO and “Cu-Sn”. Overpotential problems
caused by this effect could also explain the initial low discharge plateau (-200 mV) of
some of the Li2CuSn cells. It appears that the delithiation process produces a mix of
finely divided tin, and the bronze @&s then proceeds along the reaction pathway stated
above. For all of these Cu-Sn materials, it appears that the initial lithiation of the alloy
results in the decomposition of the material to form a matrix of active Sn in inactive Cu.
Copper-tin interrnetallic materials have been investigated as anode materials to
replace carbon in lithium-ion cells. This initial study has demonstrated the strong effect
that an inactive matrix element can have on the utilization of the active Sn component.
Some improvement in the cycling of these materials over pure tin was also observed.
Support from the Advanced Battery Program, Chemical Sciences Division, OffIce
of Basic Energy Sciences, US Department of Energy under contract no. W-3 l-109-Eng-
38 is gratefully acknowledged.
1. G. Pistoia, Lithium Batteries, New Materials, Developments, and Perspectives,
Industrial Chemistry Library, Vol. 5, Elsevier, Amsterdam (1994).
2. J. Wang, I. D. Raistrick, and R. A. Huggins, J. Electrochem. Sot. 133,457 (1986).
-. . .. ,, .,., ., .?,.,.,. . !,. . ,.-7. ., -., ,. -. . .. . . . . ., . . . . . ., . .. . ..<....>. ... ,,
3. Y. Idota, T. Kubota, A. Matsufuji, Y. Maekawa, and T. Miyasaka, Science 276,
4, I. A. Courtney and J. Dahn, J. Electrochem. Sot. 144,2045 (1997).
5. V. V. Pavlyuk, 0.1. Bodak, and G. S. Dmytriv, Ukr. Khim. Zh. 58,735 (1992).
6. C. S. Johnson, D. W. Dees, M. F. Mansuetto, M. M. Thackeray, D. R. Vissers, D.
Argyriou, C.-K. Loong and L. Christensen, J. Power Sources, 68,570 (1997).
--.-~- --.. :.:,,,, ,..,, ~J!< ,%+ . . (, . . . ,.;... .;-, , ., ~--- ,,—.. -.— .-- —..
,., -—--, - .—---
Fig. 1. The structure of Cu@ns.
Captions to Figures
The black spheres represent the trigonal prismatic
coordination of the tin site, while the gray spheres represent the copper, which has
Fig. 2. The electrochemical profiles of the f~st discharge and subsequent charge of a
typical (a) Li/Sn cell, and (b) Li/cU6fh15 cell, and (c) the charge and subsequent
discharge of a typical Li/LizCuSn cell.
Fig. 3. Capacity vs. cycle number for Li/Sn, LizCuSn, and Li/cU6sn5+& (8 = 0, *1) cells
over the range 1.2 – 0.0 V (20 cycles).
Fig. 4. Cell capacity in mAh/(g Sn) vs. cycle number for Li/Sn and Li/cU6h5+& (~= O,*1)
cells cycled over the range 1.2 to 0.0 V (20 cycles).
Fig. 5. Cell capacity vs. cycle number for Li/Sn and Li/Cu&ns+5(8=0, M) cells cycled
over the range 1.2 to 0.2 V (20 cycles).
Fig. 6. The structure of L12CuSn. In this material, lithium-cations occupy the interstitial
sites created within a copper (gray spheres) and tin (black spheres) metal array.
.—.. .— ., .... -L-Y. ,-. ——-. . . . . .
.. . —= ..— —....—— - -... ..
II I /I I I
0.2- !11, /’ ,
I0. T , 1 , I 1
0 10 20 30 40 50
o 10 20 30 40 50 60
0 5 10 15 20
R \ 1-
.....o ..0.. .+
-x-----~%--- ““-$ 0 ......
‘“ +.. - ...+ ......+. .,,.*, ‘
v““‘“--+-. ... . ,,+ -.,
II i I 1 1 I 1 I I
o 2 4 6 8 10 12 14 16 18’:
Q Cu6Sn4\ A ‘+%.
I [ 1 I I I 1 I i
o 2 4 6 8 10 12 14 16 18 2(
. . ... . ~r——— .= - -,-. .-—, ----- -. ----.—–- -
. ...7.......r r.,.- ,,. ,.m ,,-. ,., , ,. .-,+ ,>,..< .,++, .>- .~ce.;~.7-- ~ .. . . . ,,. . --—- —-- -